#------------------------------------------------------------------------------
#$Date: 2016-03-26 13:46:54 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180235 $
#$URL: svn://www.crystallography.net/cod/cif/7/11/21/7112155.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7112155
loop_
_publ_author_name
'Teresa Eaton'
'Jian Lin'
'Justin N. Cross'
'Jared T. Stritzinger'
'Thomas E. Albrecht-Schmitt'
_publ_section_title
;
 Th(VO3)2(SeO3) and Ln(VO3)2(IO3) (Ln = Ce, Pr, Nd, Sm, and Eu): unusual
 cases of aliovalent substitution
;
_journal_name_full               Chem.Commun.
_journal_page_first              3668
_journal_paper_doi               10.1039/c4cc00537f
_journal_volume                  50
_journal_year                    2014
_chemical_formula_moiety         Eu(VO3)2(IO3)
_chemical_formula_sum            'Eu I O9 V2'
_chemical_formula_weight         524.74
_chemical_melting_point          ?
_chemical_name_common            'Europium vanadate iodate'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           57
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2c 2b'
_symmetry_space_group_name_H-M   'P b c m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   6.9278(4)
_cell_length_b                   14.2624(9)
_cell_length_c                   7.1720(5)
_cell_measurement_reflns_used    1522
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.56
_cell_measurement_theta_min      2.86
_cell_volume                     708.64(8)
_computing_cell_refinement       'smart saint'
_computing_data_collection       smart
_computing_data_reduction        saint
_computing_molecular_graphics    'SHELXS-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXS-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'BRUKER apex II'
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_radiation_monochromator  'Quazar optics'
_diffrn_radiation_source         'Imus microfocused'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0337
_diffrn_reflns_av_sigmaI/netI    0.0149
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            10426
_diffrn_reflns_theta_full        27.56
_diffrn_reflns_theta_max         27.56
_diffrn_reflns_theta_min         2.86
_exptl_absorpt_coefficient_mu    15.705
_exptl_absorpt_correction_T_max  0.882
_exptl_absorpt_correction_T_min  0.860
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   shelxprep
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    4.918
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Columnar
_exptl_crystal_F_000             936
_exptl_crystal_size_max          0.01
_exptl_crystal_size_mid          0.008
_exptl_crystal_size_min          0.008
_refine_diff_density_max         2.085
_refine_diff_density_min         -0.925
_refine_diff_density_rms         0.186
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.114
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     71
_refine_ls_number_reflns         885
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.111
_refine_ls_R_factor_all          0.0183
_refine_ls_R_factor_gt           0.0155
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0182P)²+1.2728P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0343
_refine_ls_wR_factor_ref         0.0350
_reflns_number_gt                832
_reflns_number_total             885
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4cc00537f2.cif
_cod_data_source_block           EuV2I2O9
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'N/A' was changed to '?' - the value
is undefined or not given.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'N/A' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      Pbcm
_cod_database_code               7112155
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x, y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Eu1 Eu 0.85213(3) 0.046080(15) 0.2500 0.00325(8) Uani 1 2 d S
I1 I 1.29844(4) -0.05382(2) 0.2500 0.00376(8) Uani 1 2 d S
V1 V 0.45899(11) -0.2500 0.0000 0.00302(16) Uani 1 2 d S
V2 V 0.81869(11) -0.22789(5) 0.2500 0.00295(16) Uani 1 2 d S
O1 O 1.1732(3) 0.01273(15) 0.0687(3) 0.0045(4) Uani 1 1 d U
O2 O 1.5285(5) 0.0021(2) 0.2500 0.0096(7) Uani 1 2 d S
O3 O 0.3225(3) -0.15774(16) -0.0487(3) 0.0063(5) Uani 1 1 d .
O4 O 0.5266(4) -0.2827(2) -0.2500 0.0046(6) Uani 1 2 d S
O5 O 0.7380(4) -0.2500 0.0000 0.0059(7) Uani 1 2 d S
O6 O 0.9893(5) -0.3074(2) 0.2500 0.0057(6) Uani 1 2 d S
O7 O 0.9214(5) -0.1233(2) 0.2500 0.0047(6) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Eu1 O6 133.35(12) 1_455 3_755
O2 Eu1 O3 72.65(9) 1_455 2_655
O6 Eu1 O3 69.92(8) 3_755 2_655
O2 Eu1 O3 72.65(9) 1_455 5_655
O6 Eu1 O3 69.92(8) 3_755 5_655
O3 Eu1 O3 71.66(10) 2_655 5_655
O2 Eu1 O7 85.60(11) 1_455 .
O6 Eu1 O7 141.04(11) 3_755 .
O3 Eu1 O7 136.79(6) 2_655 .
O3 Eu1 O7 136.79(6) 5_655 .
O2 Eu1 O1 80.69(6) 1_455 5_755
O6 Eu1 O1 109.73(5) 3_755 5_755
O3 Eu1 O1 137.29(7) 2_655 5_755
O3 Eu1 O1 68.81(7) 5_655 5_755
O7 Eu1 O1 71.15(5) . 5_755
O2 Eu1 O1 80.69(6) 1_455 2_755
O6 Eu1 O1 109.73(5) 3_755 2_755
O3 Eu1 O1 68.81(7) 2_655 2_755
O3 Eu1 O1 137.29(7) 5_655 2_755
O7 Eu1 O1 71.15(5) . 2_755
O1 Eu1 O1 138.89(10) 5_755 2_755
O2 Eu1 O1 140.23(7) 1_455 6_556
O6 Eu1 O1 76.45(8) 3_755 6_556
O3 Eu1 O1 104.06(7) 2_655 6_556
O3 Eu1 O1 145.49(7) 5_655 6_556
O7 Eu1 O1 69.91(8) . 6_556
O1 Eu1 O1 117.60(5) 5_755 6_556
O1 Eu1 O1 62.22(8) 2_755 6_556
O2 Eu1 O1 140.23(7) 1_455 .
O6 Eu1 O1 76.45(8) 3_755 .
O3 Eu1 O1 145.49(7) 2_655 .
O3 Eu1 O1 104.06(7) 5_655 .
O7 Eu1 O1 69.91(8) . .
O1 Eu1 O1 62.22(8) 5_755 .
O1 Eu1 O1 117.60(5) 2_755 .
O1 Eu1 O1 59.51(10) 6_556 .
O2 Eu1 I1 139.63(9) 1_455 .
O6 Eu1 I1 87.02(8) 3_755 .
O3 Eu1 I1 135.69(5) 2_655 .
O3 Eu1 I1 135.69(5) 5_655 .
O7 Eu1 I1 54.02(8) . .
O1 Eu1 I1 85.49(5) 5_755 .
O1 Eu1 I1 85.49(5) 2_755 .
O1 Eu1 I1 32.11(5) 6_556 .
O1 Eu1 I1 32.11(5) . .
O2 Eu1 I1 74.876(11) 1_455 5_755
O6 Eu1 I1 95.95(2) 3_755 5_755
O3 Eu1 I1 113.94(5) 2_655 5_755
O3 Eu1 I1 44.13(5) 5_655 5_755
O7 Eu1 I1 94.78(2) . 5_755
O1 Eu1 I1 24.69(5) 5_755 5_755
O1 Eu1 I1 152.72(5) 2_755 5_755
O1 Eu1 I1 135.95(5) 6_556 5_755
O1 Eu1 I1 76.47(5) . 5_755
I1 Eu1 I1 105.422(5) . 5_755
O2 Eu1 I1 74.877(11) 1_455 5_756
O6 Eu1 I1 95.95(2) 3_755 5_756
O3 Eu1 I1 44.13(5) 2_655 5_756
O3 Eu1 I1 113.94(5) 5_655 5_756
O7 Eu1 I1 94.78(2) . 5_756
O1 Eu1 I1 152.72(5) 5_755 5_756
O1 Eu1 I1 24.69(5) 2_755 5_756
O1 Eu1 I1 76.47(5) 6_556 5_756
O1 Eu1 I1 135.95(5) . 5_756
I1 Eu1 I1 105.422(5) . 5_756
I1 Eu1 I1 147.391(11) 5_755 5_756
O2 I1 O1 101.07(11) . .
O2 I1 O1 101.07(11) . 6_556
O1 I1 O1 90.63(14) . 6_556
O2 I1 Eu1 128.68(11) . .
O1 I1 Eu1 49.60(7) . .
O1 I1 Eu1 49.60(7) 6_556 .
O2 I1 Eu1 103.677(19) . 5_755
O1 I1 Eu1 33.88(7) . 5_755
O1 I1 Eu1 122.32(7) 6_556 5_755
Eu1 I1 Eu1 74.579(5) . 5_755
O2 I1 Eu1 103.677(19) . 5_756
O1 I1 Eu1 122.32(7) . 5_756
O1 I1 Eu1 33.88(7) 6_556 5_756
Eu1 I1 Eu1 74.579(5) . 5_756
Eu1 I1 Eu1 147.391(11) 5_755 5_756
O3 V1 O3 110.42(16) 4_545 .
O3 V1 O4 97.82(12) 4_545 7_556
O3 V1 O4 98.25(12) . 7_556
O3 V1 O4 98.25(12) 4_545 .
O3 V1 O4 97.82(12) . .
O4 V1 O4 151.64(19) 7_556 .
O3 V1 O5 124.79(8) 4_545 .
O3 V1 O5 124.79(8) . .
O4 V1 O5 75.82(9) 7_556 .
O4 V1 O5 75.82(9) . .
O3 V1 V2 120.13(8) 4_545 7
O3 V1 V2 114.80(8) . 7
O4 V1 V2 111.86(9) 7_556 7
O4 V1 V2 39.84(9) . 7
O5 V1 V2 36.151(12) . 7
O3 V1 V2 114.80(8) 4_545 .
O3 V1 V2 120.13(8) . .
O4 V1 V2 39.84(9) 7_556 .
O4 V1 V2 111.86(9) . .
O5 V1 V2 36.150(12) . .
V2 V1 V2 72.30(2) 7 .
O7 V2 O6 108.31(16) . .
O7 V2 O5 106.01(5) . .
O6 V2 O5 95.58(8) . .
O7 V2 O5 106.01(4) . 6_556
O6 V2 O5 95.58(8) . 6_556
O5 V2 O5 140.62(15) . 6_556
O7 V2 O4 111.20(15) . 7_556
O6 V2 O4 140.49(15) . 7_556
O5 V2 O4 73.72(9) . 7_556
O5 V2 O4 73.72(9) 6_556 7_556
O7 V2 V1 116.08(9) . 6_556
O6 V2 V1 120.80(9) . 6_556
O5 V2 V1 107.05(9) . 6_556
O5 V2 V1 36.78(9) 6_556 6_556
O4 V2 V1 37.10(3) 7_556 6_556
O7 V2 V1 116.08(9) . .
O6 V2 V1 120.80(9) . .
O5 V2 V1 36.78(9) . .
O5 V2 V1 107.05(9) 6_556 .
O4 V2 V1 37.10(3) 7_556 .
V1 V2 V1 71.04(2) 6_556 .
I1 O1 Eu1 121.43(11) . 5_755
I1 O1 Eu1 98.29(9) . .
Eu1 O1 Eu1 117.78(8) 5_755 .
I1 O2 Eu1 169.1(2) . 1_655
V1 O3 Eu1 156.29(13) . 5_655
V1 O4 V1 139.52(17) 6 .
V1 O4 V2 103.06(10) 6 7
V1 O4 V2 103.06(10) . 7
V2 O5 V2 145.87(18) 7 .
V2 O5 V1 107.07(9) 7 .
V2 O5 V1 107.07(9) . .
V2 O6 Eu1 161.52(19) . 3_745
V2 O7 Eu1 143.28(18) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 O2 2.328(3) 1_455
Eu1 O6 2.361(3) 3_755
Eu1 O3 2.467(2) 2_655
Eu1 O3 2.467(2) 5_655
Eu1 O7 2.462(3) .
Eu1 O1 2.441(2) 5_755
Eu1 O1 2.441(2) 2_755
Eu1 O1 2.620(2) 6_556
Eu1 O1 2.620(2) .
Eu1 I1 3.4045(4) .
Eu1 I1 3.7363(3) 5_755
Eu1 I1 3.7363(3) 5_756
I1 O2 1.782(3) .
I1 O1 1.829(2) .
I1 O1 1.829(2) 6_556
I1 Eu1 3.7363(3) 5_755
I1 Eu1 3.7363(3) 5_756
V1 O3 1.658(2) 4_545
V1 O3 1.658(2) .
V1 O4 1.9110(11) 7_556
V1 O4 1.9110(11) .
V1 O5 1.933(3) .
V1 V2 3.0861(9) 7
V1 V2 3.0861(9) .
V2 O7 1.653(3) .
V2 O6 1.638(3) .
V2 O5 1.9044(9) .
V2 O5 1.9044(9) 6_556
V2 O4 2.030(3) 7_556
V2 V1 3.0861(9) 6_556
O1 Eu1 2.441(2) 5_755
O2 Eu1 2.328(3) 1_655
O3 Eu1 2.466(2) 5_655
O4 V1 1.9110(11) 6
O4 V2 2.030(3) 7
O5 V2 1.9044(9) 7
O6 Eu1 2.361(3) 3_745
